1.
View Online PAPER www.rsc.org/pccp | Physical Chemistry Chemical Physics A solid-state NMR and DFT study of compositional modulations in AlxGa1ÀxAsw Paulus J. Knijn,a P. Jan M. van Bentum,a Ernst R. H. van Eck,a Changming Fang,a Dennis L. A. G. Grimminck,a Robert A. de Groot,a Remco W. A. Havenith,a Martijn Marsman,b W. Leo Meerts,a Gilles A. de WijsaDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 and Arno P. M. Kentgens*a Received 25th February 2010, Accepted 17th May 2010 DOI: 10.1039/c003624b We have conducted 75As and 69Ga Nuclear Magnetic Resonance (NMR) experiments to Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B investigate order/disorder in AlxGa1ÀxAs lift-oﬀ ﬁlms with x B 0.297 and 0.489. We were able to identify all possible As(AlnGa4Àn) sites with n = 0–4 coordinations in 75As NMR spectra using spin-echo experiments at 18.8 Tesla. This was achieved by employing high rf ﬁeld strengths using a small solenoid coil and an NMR probe speciﬁcally designed for this purpose. Spectral deconvolution, using an evolutionary algorithm, complies with the absence of long-range order if a CuAu based order parameter is imposed. An unconstrained ﬁt shows a deviation of the statistics imposed by this type of ordering. The occupational disorder in the Ga and Al positions is reﬂected in a distribution of the Electric Field Gradients (EFGs) experienced at the diﬀerent arsenic sites. We established that this can be modelled by summing the eﬀects of the ﬁrst coordination sphere and a Czjzek type distribution resulting from the compositional variation in the Al/Ga sub-lattice in the higher coordination spheres. 69Ga 3QMAS and nutation data exclude the presence of highly symmetric sites and also show a distribution in EFG. The experimentally obtained quadrupolar interactions are in good agreement with calculations based on Density Functional Theory (DFT). Using additivity of EFG tensors arising from distant charge perturbations, we could use DFT to model the EFG distributions of the n = 0–4 sites, reproducing the Czjzek and extended Czjzek distributions that were found experimentally. On the basis of these calculations we conclude that the 75As quadrupolar interaction is sensitive to compositional modulations up to the 7th coordination shell in these systems. Introduction positive excess enthalpy, these structures can order metastably in bulk and can become stable in epitaxially grown ﬁlms. Other Thin ﬁlm semiconductors are of great importance for electronic crystallographic arrangements such as the CuPt structure do not and photonic devices. The development of new or improved possess enough geometrical degrees of freedom to permit all devices relies on a detailed knowledge of the structural properties chemical bonds to attain their ideal length, and are therefore of the materials. In this respect compositional modulation and unstable. Nevertheless, ordering of alternating diagonal planes ordering play an important role. As was predicted by Zunger in the h111i direction was found experimentally which was and coworkers1 in the mid eighties, long-range order can occur explained by assuming atomic dimerization at the surface, in semiconductor alloys with size-mismatched constituents, inducing CuPt ordering in the subsurface layers.4 despite the fact that the mixing enthalpy is positive. This can As there is hardly any size-mismatch in AlGaAs, long-range be explained by the fact that the statistical average over the order has not been widely observed. Nevertheless, Krahmer many diﬀerent local environments is positive, because some of et al.5 reported evidence of a direct–indirect conduction band these clusters are strained. Periodically repeating a three- transition for x = 0.4 in AlxGa1ÀxAs by using reﬂectance dimensional geometric re-arrangement can minimize strain anisotropy spectrometry, indicating an increase in order. They and leads to long-range order. These predictions were soon report that doping, temperature and substrate orientation all veriﬁed by experimental observations of ordering in semi- aﬀect the anisotropy of the lattice, but did not quantify this in conductors by Stringfellow and coworkers2 and Gomyo and terms of an order parameter. X-ray measurements from Kuan6 Suzuki.3 For many III–V compounds the ordered phase has et al. reported a low long-range order parameter S o 0.5 for a Al0.75Ga0.25As grown by MOCVD, depending on growth Institute for Molecules and Materials, Radboud University Nijmegen, Toernooiveld 1, NL-6525 ED Nijmegen, The Netherlands conditions. More recent X-ray measurements by van Niftrik b Institut fu¨r Materialphysik and Centre for Computational Materials et al.7 indicated a lower long-range ordering of S r 0.05 for Science, Universita Wien, A 1090, Wien, Austria ¨t Al0.5Ga0.5As and S r 0.06 for Al0.25Ga0.75As. Despite the w Electronic supplementary information (ESI) available: Additional prediction of almost no long-range ordering with X-ray, information including an experimental NMR section concerning the QCPMG data and a theoretical DFT part. See DOI: 10.1039/ studies of the local interface for dilute AlGaAs with cross- c003624b sectional STM (XSTM) indicate the appearance of short This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
2.
View Online strings. In 1994, an XSTM study by Smith et al.8 conﬁrmed order of nq = 3Cq/(2I(2I À 1)) whereas the shape of the that an interrupted growth process can create short period observed patterns reﬂects the asymmetry parameter Z of the super lattices in AlGaAs. In 1996, Smith et al.9 noticed a interaction. The central transition, h1/2;À1/2i is not aﬀected small deviation from random ordering in the Al–Al pair by the quadrupolar interaction in ﬁrst order but the second- distributions at the interface of GaAs and Al0.05Ga0.95As. order features are dispersed over a frequency range of the In 1999, Heinrich et al.10 clearly observed strings of Al order of n2 /n0, where the shape is again characteristic for the q atoms in the GaAs matrix, up to ﬁve atoms in MOVPE asymmetry of the EFG tensor. Even at high external ﬁelds thisDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 grown Al0.15Ga0.85As along low indexed crystallographic second-order interaction can result in MHz bandwidths for directions. nuclei such as 75As. To excite such a bandwidth eﬃciently, In general, the composition of III–V semiconductors is suﬃciently large rf ﬁeld strengths are needed. In relation to diﬃcult to describe since various structural features can exist this one has to realize that the behavior of the spin system in (simultaneously) at diﬀerent length scales. For instance, the the rotating frame during rf-irradiation depends on the ratio presence of both ordered and disordered domains makes it of the quadrupolar frequency and the rf ﬁeld strength.12,13 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B hard to analyze these structures in detail. The degree of order Therefore, the eﬀective excitation of the spin systems has to be will aﬀect many physical and electronic properties such as modeled accurately, especially when quantitative results electronic transport, mobility, thermodynamic stability and of diﬀerent spin systems with widely diﬀering quadrupolar electro-optical properties. Many properties of AlGaAs are parameters are needed. Additionally, with such diﬀerent sites described in detail in the work of Adachi.11 Considering the present spectral overlap will often occur, demanding a robust limited number of reports on long-range order in AlGaAs thin approach to spectral deconvolution. Finally, to interpret ﬁlms as studied by diﬀraction techniques, whereas speciﬁc NMR spectra in relation to structures, a ﬁrst principle ordered structures are seen in a number of microscopic approach such as DFT is desirable. observations, it is interesting to study these materials with In the present contribution we address all of the issues a complimentary method such as NMR. As NMR probes described above. Using small rf-coils it is possible to generate short-range order, the presence of locally occurring structures appropriate rf-ﬁelds to excite a broad bandwidth. These coils can be detected if present in suﬃciently high concentrations. also help in overcoming the sensitivity problems related Since the NMR signal is composed out of contributions from to the study of thin ﬁlm materials leading to very low the entire sample, the possibility that one is studying a speciﬁc quantities of sample material.14 Here we compare spin-echo anomaly is reduced. Long-range ordered structures will result experiments and frequency-stepped Quadrupolar Carr–Purcell– in a speciﬁc signature which can be directly distinguished from Meiboom–Gill (QCPMG)15–18 experiments to obtain static 75 a disordered structure. As spectra of two AlGaAs ﬁlms with diﬀerent composition. NMR is a versatile technique that in principle can detect all Spectral deconvolution and quantiﬁcation of the spectra is nuclei which possess a spin through their interaction with an addressed with a dedicated program based on an evolutionary external magnetic ﬁeld (the Zeeman interaction). A number of algorithm. 69Ga 3QMAS19 and nutation12,13 NMR spectra interactions make NMR useful as they give the spectra a have been obtained to gain complementary information about speciﬁc appearance which can be related to local structure the local symmetry of the diﬀerent lattice sites. Although and dynamics of the material under study. In the present work this work focuses on AlGaAs thin ﬁlm materials, the two of these are important; the chemical shift and the approach presented can be applied for the investigation of quadrupolar interaction. The external magnetic ﬁeld used in compositional modulations in most III–V semiconductors NMR induces local ﬁelds in molecules and materials that and materials with related variations in the occupancy of modify the resonance frequencies and makes diﬀerent sites diﬀerent lattice positions, sometimes called substitutional distinguishable, this is referred to as the chemical shift. For a disorder. I 4 1/2 nucleus, the quadrupolar interaction arises from the Furthermore, we develop a modeling approach to accurately presence of an electric ﬁeld gradient (EFG), resulting from the describe the EFG distributions of various kinds of sites. To local charge distribution around the site of a nucleus which this end we extended the ﬁrst-principles DFT code of interacts with the non-spherically symmetric charge distribution VASP (Vienna Ab initio Simulation Program), to calculate of that nucleus. Although NMR is an appealing technique that EFGs and build a model wherein we can quickly calculate may form a bridge between diﬀraction studies and microscopic the EFGs for several millions of conﬁgurations based on observations in the study of III–V semiconductors, there are a just one DFT calculation. This model is used to estimate number of challenges that have to be addressed. Many nuclei the sensitivity of EFGs to variations in the order parameter. encountered in III–V semiconductors are quadrupolar nuclei, It has a wider scope, as it in principle provides the capability possessing a large quadrupolar moment eÁQ. The strength of to quickly obtain electronic density distributions for the interaction expressed through the quadrupole coupling any structural model for any ‘‘random’’ alloy with ﬁxed sub- constant Cq = e2qQ/h can be very large, easily in the tens of lattices. MHz regime. Although this interaction can still be treated as perturbation of the Zeeman Hamiltonian, if suﬃciently high Studying (dis-)order with NMR external ﬁelds are applied, the quadrupolar interaction has, in general, to be treated as a second-order perturbation. Based on theory used to analyze diﬀraction data, an order To ﬁrst-order the spectral features of the so-called satellite parameter S can be deﬁned to quantify the degree of transitions are dispersed over a wide frequency range of the long-range order related to the fractional occupancy of lattice Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
3.
View Online sites by their preferred atom.6 S = 0 represents a completely pCuPt = 3(1 À rB)rA(1 À rA)2 + 3rA(1 À rB)rB2 2 2 2 random structure and S = 1 corresponds to a completely + 3(1 À rB)2rB(1 À rA) + 3rA2(1 À rA)rB ordered lattice: 2 2 S = |rA + rB À 1|, (1) pCuPt = 1rA3rB + 1(1 À rB)3(1 À rA) + 3rA2(1 À rB)(1 À rA) 3 2 2 2 where rA and rB are the fractions of A and B lattice sites that + 3(1 À rB)2rArB 2 are occupied by their preferred atom. For binary systems, as pCuPt = 1(1 À rB)rA3 + 1rA(1 À rB)3Downloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 considered here, this means that 1 À rA constitutes the fraction 4 2 2 (5) of A lattice sites occupied by B atoms and 1 À rB the fraction of B sites occupied by A atoms. In case of random occupation of pCuAu = (1 À rA)2rB2 0 the lattice sites, i.e. the absence of ordering, rA = x and rB = 1 À x. For (partially) ordered structures the fractional pCuAu = 2rA(1 À rA)rB2+2(1 À rB)(1 À rA)2rB 1 occupancy of the A and B sites by their preferred atoms can be Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B re-written as: pCuAu = rA2rB2+(1 À rB)2(1 À rA)2 +4rA(1 À rB)rB(1 À rA) 2 rA = x + S/2 (2) rB = (1 À x)+S/2 (3) pCuAu = 2rA2(1 À rB)rB+2rA(1 À rB)2(1 À rA) 3 Using this deﬁnition we should realize that the order para- pCuAu = (1 À rB)2rA2 4 (6) meter S can reach a value of 2x at most. A perfectly ordered structure can only be achieved for x = 0.5. S can be scaled, however, so that the maximum possible order As the probabilities correspond to the integrated peak for any given composition x gives an order parameter intensities of the diﬀerent sites, one can determine the long- S = 1.20 range order parameter by drawing the experimental peak The presence of (dis-)order in a structure is in most cases intensities in a plot of calculated intensities versus order manifested in quantiﬁable NMR parameters. Diﬀerent parameter S. Using the relative 31P peak intensities Tycko structural environments in a material can be distinguished et al.22 were able to set an upper limit of S o 0.6 for the CuPt based on the NMR interactions which are inﬂuenced by the type ordering in InGaP. Degen et al.21 observed the 75As diﬀerent coordinating atoms. For example, Tycko et al.22 resonances of the locally symmetric As[Al4] and As[Ga4] distinguished ﬁve 31P sites in the 31P MAS NMR spectrum coordinations in static single-pulse excitation experiments on of GaInP. These ﬁve resonances were assigned to the diﬀerent powdered AlGaAs ﬁlms. They were able to set an upper limit phosphorus nearest neighbors coordinations P[In4ÀnGan] with of S o 0.2 and S o 0.4 for CuAu and CuPt ordering n = 0–4. The sites are resolved in this spectrum due to their respectively. Although spin-echo experiments hinted at the diﬀerent isotropic chemical shifts. The presence of order in the presence of the other 75As coordinations, these proved to be sample is reﬂected in the statistics of the occurrence of the various too broad to be eﬃciently excited and resolved in the coordinations.21,22 The probabilities pn for the occupations of spectrum. the C[AnB4Àn] sites are Finding low values for the long range order parameter S indicates that the atomic distribution of A and B atoms p0 = pC[B4] becomes more or less random over their lattice positions. It may well be, however, that there is still a preference for local p1 = pC[A1B3] p2 = pC[A2B2] p3 = pC[A3B1] p4 = pC[A4] (4) Here, two types of ordering are considered for AxB1ÀxC type materials, see Fig. 1. CuPt ordering, with diagonal planes, stacked in the h111i direction or a CuAu, with alternating Fig. 1 Order in the face centered cubic lattice structure of AlGaAs. planes in h001i. For each conﬁguration, we can quantify the The black atoms are Arsenic, the other atoms are the Al and Ga probability of their occurrence. The 16 possible atomic con- cations. left 2-fold symmetry of the As nucleus for a AsAl2Ga2 ﬁgurations in the ﬁrst shell contribute each with a diﬀerent conﬁguration, CuAu ordered with planes alternating along the h001i probability: direction. right 3-fold tetrahedral symmetry of the As nucleus for a AsAl3Ga and AsAlGa3 conﬁguration, also called CuPt ordered lattice pCuPt = 1rB(1 À rA)3 + 1(1 À rA)rB3 0 2 2 with planes extending along the h111i direction. Coordination numbers and distances are 0.40 and 0.245 nm for the ﬁrst coordination pCuPt = 1(1 À rB)(1 À rA)3 + 1rArB3 + 3rArB(1 À rA)2 sphere, 1.20 and 0.40 nm for the second coordination sphere and 1.20 1 2 2 2 and 0.469 nm for the third coordination sphere. The lattice constant is + 3(1 À rB)(1 À rA)rB2 2 Ax = 0.566140 À 0.000809Áx nm.21 This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
4.
View Online ordering of Al and Ga in the sample, e.g., when A atoms prefer can be obtained but this approach is still not satisfactory as Cq B atoms in their vicinity and vice versa. Alternatively, atoms and Z are treated independently, needing a starting value for Z. can show a tendency to be close neighbors which is referred to Moreover, the distribution is generated numerically lacking an as clustering. Short-range ordering and clustering is very analytical description. diﬃcult to detect with diﬀraction techniques as they cause A physically more sound model for describing the distribution only very weak diﬀuse scattering. In NMR the statistics of the of electric ﬁeld gradients in amorphous solids has been developed diﬀerent coordinations will be modulated by either short range by Czjzek et al.25 They proposed a joint probability densityDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 order or clustering, which should be expressed in increased function numbers for p0 or p4. The exact eﬀect and size of the variations will depend on the scale and abundance of the locally 2 ÀVzz ð1 þ Z2 =3Þ ordered structures and may be diﬃcult to interpret depending PðVzz ; ZÞ ¼A Á exp 2s2 on the accuracy with which the spectral line intensities can be ð7Þ determined. V dÀ1 Á Zð1 À Z2 =9Þ A ¼ zz pﬃﬃﬃﬃﬃﬃ ; Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B Besides modulating the intensities of the various C[AnB4Àn] 2psd resonances in the spectra it should be realized, however, that the distribution of A and B atoms over the lattice also aﬀects in which the average quadrupolar coupling constant depends the NMR parameters such as the chemical shift and the on s and d, see Table 1. In this work, we show that for a quadrupolar interaction parameters nq and Z of these sites. randomly ordered lattice, the quadrupolar distributions Especially for the quadrupolar interaction it is important to caused by a random occupancy of the A and B sites over consider that the interaction is not fully determined locally. the lattice can be described by a Czjzek distribution with Although the electric ﬁeld gradient tensor is dominated by the d = 5 for the symmetric C[A4] and C[B4] sites. These ﬁrst shell bonds, further coordination shells still have a distinct distributions are isotropic and rotation invariant. Eqn (7) is inﬂuence. This is witnessed by the fact that the symmetric derived from the fact that the real terms Um(m = 0–4) (deﬁned ﬁrst shell As coordinations, As[Al4] and As[Ga4], observed in references)25,26 of the EFG tensor are independently, by Degen et al.21 in AlGaAs, show non-zero quadrupolar normally distributed variables for amorphous solids with interactions with quadrupolar coupling constants of 800 and random ionic coordinations. The ﬁve independent spherical 600 kHz respectively. tensor elements Vi,k of the EFG tensor are linear combinations Structural disorder leads to distributions in chemical shift of these Um. A similar approach was introduced by Stock- ¨ and quadrupolar interactions, which aﬀect the measured line mann27 describing the eﬀect of randomly distributed defects in shapes in a characteristic way. Therefore, a detailed study of cubic crystals. the line shapes in disordered solids can be interpreted in terms As was outlined by Massiot and coworkers,28 the Czjzek of structural variations in these materials if one can extract the distribution can only be used if the number of structural probability density function for the quadrupolar interaction elements contributing to the EFG is suﬃciently large, meaning parameters from the spectra and compute the EFG tensors for that for a given coordination shell the coordination number a given structure, e.g., based on ﬁrst principles DFT based should be large. This will in general not be the case for the ﬁrst calculations. coordination shell. Therefore the Czjzek distribution can in Extraction of the probability density function from NMR principle only be used if the ﬁrst coordination sphere hardly spectra of randomly oriented powder samples is not trivial contributes to the EFG as is the case for the symmetric as the distribution in quadrupolar NMR parameters is As[Al4] and As[Ga4] sites in AlGaAs or the octahedrally and convoluted with the powder averaging over all possible tensor tetrahedrally coordinated aluminium sites discussed by orientations in the ensemble. In the NMR literature several Massiot et al.28 Clearly, the ﬁrst coordination sphere dominates approaches to model the probability density function(s) for the EFG for the asymmetric As[AlnGa4Àn] sites with n = 1,2,3 the quadrupolar interaction parameters can be found. The in AlGaAs. To deal with this situation an extension of the most basic approach is to assume Gaussian distributions Czjzek approach is needed, considering the case of an EFG in Cq and Z. Although such distributions are not physically contribution of a well-deﬁned local coordination of a given justiﬁed they regularly do produce line shapes similar to the atomic species and adding to that the eﬀect of disorder of more experimental ones and can therefore be used in spectral remote atomic shells and possible other random contributions deconvolutions in order to properly quantify the relative line to the total EFG. Due to the good lattice matching of the intensities. One should be careful with interpreting these results in terms of structural disorder, however, especially where the asymmetry parameter Z is concerned. First of all, Table 1 The ratio of the average hVzzi to the s in a Czjzek the structural parameters are not additively described by distribution as a function of the power factor d obtained by integrating eqn (7) over all Z for a given s quadrupolar parameters and are therefore not expected to be normally distributed and moreover nq and Z are coupled as d hVzzi/s they both depend on the local electronic coordination around 1 0.74 a nucleus. Jager et al.23 and Meinhold et al.24 have improved ¨ 2 1.17 on this basic model by assuming normal distributions in the 3 1.49 eigenvalues of the EFG tensor and applying constraints to 4 1.76 5 2.00 warrant the tracelessness of this tensor. Again good line shapes Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
5.
View Online AlGaAs lattice, we neglect any stress in the lattice and propose case of a strong ﬁrst shell tensor Vzz(0) 4 40 Â 1020 V mÀ2. to use additivity for the local and remote contributions to these EFGs. This is implemented numerically by adding the ZZ ~0 ~0 U Á U ð0Þ (ﬁxed) contribution of the ﬁrst coordination shell to the Czjzek f ðVzz ; ZÞ / A Á exp 2s2 distribution resulting from (random) occupancy of Al and Ga ! lattice sites in the further coordination shells. First, the Vzz ð0Þ2 Á ð1 þ Zð0Þ2 =3Þ À Vzz Á ð1 þ Z2 =3Þ 2 principal EFG tensor values are generated from the Czjzek À dasinðbÞdbdg 2s2Downloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 distribution using Vxx = ÀVzz(Z+1)/2 and Vyy = Vzz(Z À 1)/2. The resulting tensor V is then rotated over a set of Euler angles ! ! Zð0ÞVzz ð0Þa15 using Vrot = R(a, b, g) V R(a, b, g)T, with RT the transposed U 0 Á U 0 ð0Þ ¼ 2 Á Vzz Á Vzz ð0Þa11 þ pﬃﬃﬃ 3 rotation matrix. The relative orientation is randomized by taking all possible orientations into account. The ﬁrst shell 2 Á ZVzz Zð0ÞVzz ð0Þa55 þ pﬃﬃﬃ Vzz ð0Þa51 þ pﬃﬃﬃ ; EFG is added to this tensor after which it is diagonalized and 3 3 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B sorted using Vzz Z Vxx Z Vyy. The ﬁnal distribution is ð10Þ generated by integration over all possible angles on a sphere ensuring the isotropic character of the distribution. The resulting Vzz and Z values are placed on a new grid with with Aij(a, b, g) as deﬁned in ref. 26 and A as in eqn (7). For the weights of the original Czjzek distribution. For Al2Ga2, Z(0) = 0 this equation can be written into a modiﬁed Bessel the ﬁrst shell tensor V(0) is deﬁned by a single scalar value VZ1 function form (see eqn 61 in ref. 26). Practically, the (Vzz, Z) and Z(0) = 1 distribution for Z(0) = 0 showed good overlap with the previous equation in a simpliﬁed, approximated form without 2 3 integral ÀV Z1 0 0 V¼4 0 0 0 5 ð8Þ 0 0 V Z1 Vzz Á Vzz ð0Þ f ðVzz ; ZÞ $ A Á exp 2s2 The ﬁrst shell tensor of a Al1Ga3/Al3Ga1 site is deﬁned by VZ0 ! ÀVzz ð0Þ2 Á ð1 þ Zð0Þ2 =3Þ À Vzz Á ð1 þ Z2 =3Þ 2 and Z(0) = 0 2s2 2 3 ð11Þ ÀV Z0 =2 0 0 V ¼4 0 ÀV Z0 =2 0 5 ð9Þ 0 0 V Z0 allowing a much faster calculation. The only diﬀerence with the extended Czjzek distribution that was introduced The ‘‘extended Czjzek’’ distribution generated in this way previously, is the scaling of the tensor terms and the extra y coincides with the extended Gaussian Isotropic Model parameter. Although Le Caer and Brand26 use y as a ¨ (GIM) introduced by Le Caer and Brand.26 These authors ¨ parameter for local ordering (crystalline, mixed or random give an in-depth and general discussion of models for the domains), we consider this eﬀect simply by adjusting the distributions of electric ﬁeld gradients in disordered solids. magnitude of the ﬁrst shell tensor V(0), omitting the need Their extended Gaussian Isotropic Model (GIM) considers the for an extra variable in this approach. Substituting V(0) = 0 case of an EFG tensor V0 added to a random tensor back- corresponds to the original Czjzek distribution. Very recently ˜ ˜ ground contribution VGI with a ratio y, V = (1 À y)ÁV0+yÁ Le Caer and coworkers have further developed their extension ¨ ˜ VGI. Here we assign y = 0.5, since there is an equal contribu- of the Czjzek model in view of an application to 71Ga NMR tion of the EFG tensor from the higher coordination spheres spectra of chalcogenide glasses.29 and the ﬁrst coordination shell. Since a normalization is A ﬁnal important step for interpreting distributions in ˜ missing, it is more convenient to consider V = V0 + VGI. ˜ quadrupolar NMR parameters is being able to predict the Le Caer and Brand describe the quadrupolar distribution by ¨ quadrupolar parameters on the basis of a given structural an exponential expression of three terms, integrated over a model. The calculation of EFGs using Density Functional sphere, see ref. 26, using the Euler angles a, b, g. This equation theory (DFT) has been implemented in the Full Potential is slightly modiﬁed here into eqn (10). The nominator of the Linearised Augumented Plane Wave (FLAPW) method by ~ ~ exponent consists of a mix term U 0 ÁU(0), an oﬀset term which Herzig et al.30 and in the PAW (Projector Augmented Wave) is constant Vzz(0)2Á(1 + Z(0)2/3) and merely scales the method by Petrilli et al.31 Following the latter we implemented intensities and a Czjzek term Vzz2Á(1 + Z2/3). The ‘‘ordered’’ the EFG calculation in the ﬁrst-principles electronic structure ﬁrst shell tensor has magnitude Vzz(0) and an asymmetry program VASP (Vienna Ab initio Simulation Package).32–35 parameter Z(0). In comparison with Z(0) = 0, there are two An additional challenge in this context is to appropriately ~ ~ additional cross-terms in U 0 ÁU(0), when Z(0) = 1. Even model the eﬀects of the structural variations present in the though the oﬀset term is constant, as the ratio Vzz/s can material. In case of AlGaAs, however, the eﬀects of local become large, all exponential terms need to be placed inside charge (re)distributions arising from single lattice modiﬁcations the integral and cannot be placed in front, since individually are additive, so that various disordered conﬁgurations can be the exponential terms can become extremely large 410700 in modeled with relatively low computational cost. This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
6.
View Online Experimental acquisition time was 125 ms with 7.5 ms experimental delay before and after the 1801 pulse of each echo. The individual Sample preparation 500 point whole-echos were T2 weighted before co-adding, and The AlGaAs samples were grown by Metal Organic Vapor subsequently swapped around the echo maximum and Fourier Phase Epitaxy. Undoped 2 inch GaAs wafers with crystal transformed. A more detailed description of acquisition and orientation h100i, 15 degrees oﬀ towards h111i were used as processing of the QCPMG data is given in the supplementary substrates. A typical sample consisted of a 15 nm Si-doped material.Downloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 AlAs buﬀer and a 5 mm undoped AlxGa1ÀxAs layer. A growth series with nominal aluminium fractions of x = 0, 0.297 was II. 75As Hahn-echo. Hahn-Echo experiments were produced. A sample with x = 0.489 was grown on a substrate obtained at 18.8 T, corresponding to a 75As frequency of 2 degrees oﬀ towards h110i. An epitaxial lift-oﬀ process36 was 136.93 MHz, using a Varian InﬁnityPlus Console Àp x;Àx Á applied to separate the AlxGa1ÀxAs layer from the substrate 2 À t1 À pÀy À t2 À ACQx;Àx . A recycle delay of 1 s by selectively etching the intermediate Si-doped AlAs layer was employed. Whole echoes were recorded which were Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B with a hydrogen ﬂuoride solution. The AlxGa1ÀxAs thin ﬁlms processed by swapping the data around the echo maximum (Emg quantities) were crushed into a powder with a typical followed by apodization (exponential) and zero-ﬁlling to grain size of a few micrometres and subsequently transferred 8192 points before Fourier transformation. The spectral width to plastic sample holders for NMR measurements. The sample was 5 MHz. The x E 0.297 Hahn-echo spectrum was acquired holders were made of PolyEtherEtherKeton (PEEK). with 75.000 scans and echo times of t1 = 200 ms, t2 = 75 ms and 25 ms delay from the acquisition and receiver delay. The NMR experiments 901 and the 1801 pulse times were 0.2 ms respectively 0.4 ms. 166.000 scans were averaged in the x E 0.489 Hahn-echo data A home-built, static XH probe operating at 137 MHz for with t1 = 175 ms, t2 = 5 ms and 20 ms delay from the arsenic (18.8 T) was designed for achieving high rf ﬁelds. The acquisition and receiver delay. coil was a 5-turn solenoid with a 1.2 mm internal diameter, made of a silver-plated, 220 mm diameter wire. The sample III. 69Ga Nutation and 3QMAS. A series of 69Ga static space was conﬁned to a length of 2 mm and a diameter of nutation spectra using diﬀerent rf-ﬁeld strengths were obtained 0.6 mm. The Q factor of the probe was determined to be E38. for Al0.297Ga0.703 As at 14.1 T on a Chemagnetics Inﬁnty Two Allen-Bradley 1 kO high power resistors were put parallel 600 MHz spectrometer. The same probe was used for these to the tuning capacitor to reduce the Q factor to E 20 to allow experiments, tuned to 143.99 MHz with a Q factor of B50. A frequency-stepped experiments without retuning the probe. z-ﬁltered 69Ga 3QMAS spectrum, using hyper-complex The rf-ﬁeld strength was determined by obtaining 75As nutation States TPPI,37 was recorded at 9.4 T, 96.013087 MHz, on a spectra from a sample of GaAs. In this sample As occupies a Chemagnetics Inﬁnity 400 MHz spectrometer. Here a spinning cubically symmetric lattice and therefore the signal nutates speed of 15 kHz was employed, using a Chemagnetics 2.5 mm with frequency nrf. rf ﬁeld strength up to 800 kHz were HX probe. achieved using approximately 800 Watts of power. In the QCPMG and Hahn-echo pulse experiments very short pulses IV. Spin–lattice relaxation times. To ensure quantitative are used so one has to take into account that the maximum evaluations of the spectra, spin–lattice relaxation times were voltage is never reached due to the pulse rise time depending determined for Al0.297Ga0.703As using saturation recovery on the Q factor of the probe (see supplementary material). experiments, as summarized in Table 2. The values for this Therefore actual rf ﬁelds amounted to 390 kHz and 625 kHz in x E 0.297 composition do not diﬀer strongly from the the QCPMG and Hahn-echo experiment respectively. values determined earlier21 for a sample with composition Al0.498Ga0.511As, indicating no signiﬁcant changes in relaxation I. 75As QCPMG. A well-established experiment for mechanism for diﬀerent compositions. The T1 of 75As in bulk acquiring very wide-line spectra with high sensitivity is the GaAs was 0.33 Æ 0.05 s. frequency-stepped QCPMG experiment.15–18 For such an experiment it is useful to reduce the probes’ Q factor (here Spectral deconvolution to 20). The ﬂat response of the probe minimizes the phase variations as a function of frequency. This is advantageous An important objective of this study is to characterize the 75As since the probe does not need to be re-tuned and the coordinations in AlxGa1ÀxAs and determine their relative intensity loss at large frequency oﬀsets is almost negligible. intensities. The analysis can become complex due to the presence of several overlapping resonances with a distribution 24 respectively 22 experiments were performed at 18.8 T using in NMR interaction parameters. Here we resort to ﬁtting a Varian InﬁnityPlus console. The frequency step size was 125 kHz covering a spectral width of 3 MHz for Al0.297Ga0.703As Table 2 T1(s) relaxation times obtained using saturation recovery at and Al0.489Ga0.511As. The x E 0.297 spectrum was recorded 14.1 Tesla with 10.000 scans and the x E 0.489 with 5.400 scans at each frequency step. Because T2 is long, the number of echoes Al0.297Ga0.703As Al0.489Ga0.511As21 acquired (242) was limited by experimental limitations 69 Ga — 0.77Æ0.04 71 (121.000 data points in 30 ms). The 901 and 1801 pulse times Ga 0.11Æ0.04 0.15 Æ 0.08 27 were 0.32 ms and 0.64 ms respectively. A repetition delay of 1 s Al 18 Æ 1 16.1 Æ 0.4 75 As 0.27 Æ 0.02 0.28 Æ 0.03 was used, acquiring a spectral width of 4 MHz. Each echo Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
7.
View Online procedures based on an evolutionary algorithm to provide in negligible changes (o0.002 nm) in the atom positions. All knowledge about intensities, NMR parameters and their results below were obtained using the PBE functional.44 The distribution, and the associated error margins. The program PAW datasets have frozen [Ar], [Ne] and [Ar]3d10 cores for is based on the work by Meerts38 and will be described in Ga, Al and As respectively. On the basis of these results, we detail in a forthcoming publication. The algorithm uses a think that the obtained quadrupolar distributions are a good library database of time domain data sets which were generated representation for this lattice. using SIMPSON.39,40 In this way the experimental conditionsDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 can be mimicked accurately for each experiment. For each site a group of simulated data sets are added to describe a Results and discussion distribution in interaction parameters. The weight of each 75 I. As QCPMG analysis set is determined by the selected distribution function, e.g., given by the work of Czjzek25 and Le Caer and Brand.26 For ¨ The high quadrupolar moment of 75As and its strategic anion the Hahn-echo spectra, approximately 1600 datasets were position in the AlGaAs lattice makes it the most interesting Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B generated based on the experimental rf-ﬁeld strength and nucleus to probe for information about the symmetry and bandwidth. In the simulations, the maximum of the echo ordering of the crystal lattice. As detailed in the experimental was recorded to identify the intensity contribution for each section, frequency-stepped QCPMG experiments15–18 were site. For the QCPMG spectra a slightly diﬀerent approach was used to obtain good sensitivity 75As spectra with signals followed. Calculating all echoes in a QCPMG experiment for dispersed over 2 MHz. Fig. 2 displays the summation of the each quadrupolar interaction is too time consuming and experimental QCPMG subspectra for each frequency oﬀset for therefore only a single echo was calculated assuming ideal Al0.297Ga0.703As and Al0.489Ga0.511As. The spectra show two pulses. Each subset was Fourier transformed into ﬁve absolute narrow resonances separated by d = 188 Æ 5 ppm, in simulated spectra with ideal lineshapes but including accordance with previous work45 these lines are assigned to quadrupolar distributions, which were least square ﬁtted to the signals of As[Ga4] and As[Al4] sites having a symmetric the absolute, experimental spectrum. To cover all values ﬁrst coordination sphere. An arsenic nucleus surrounded appearing in the spectra, the quadrupolar interaction by four aluminium or gallium nuclei, has a tetrahedrally parameters of the As[Ga4] and As[Al4] site were varied over symmetric structure and should therefore display no quadrupolar a range of 0 r Z r 1, 0 r Cq r 2 MHz while the As[Al2Ga2] interaction. However, depending on the positions of the site had a range of 0.9 r Z r 1, 31 r Cq r 35 MHz and cations in the third and higher coordination spheres, there the As[Al1Ga3] and As[Al1Ga3] site 0 r Z r 0.1, 31 r Cq r can still exist a (relatively small) EFG. Indeed, in the work by 35 MHz. In all ﬁts, the cost function was calculated using a Degen et al.21 a Cq = 610 kHz and Z 4 0.97 was determined normalized, least square summation for As[Ga4] and Cq = 820 kHz, Z 4 0.88 for As[Al4]. Here we show that these sites can be properly ﬁtted to a Czjzek X fi n gi 2 w2 ¼ À ; ð12Þ distribution, with d = 5 and average quadrupolar values of i¼1 fmax gmax Cq = 610 and 820 kHz, as were obtained from 75As nutation NMR experiments.21 The average quadrupolar coupling here f is the experimental spectrum and g the calculated constants for these two sites were ﬁxed as the ﬁt was not very spectrum from the library and n the number of points. The sensitive to small changes in this parameter. calculations were performed using up to 20 nodes of a high The wide resonances, not directly observed in the previous speed cluster based on Sunﬁre X4100 computers. study, show distinct quadrupolar features of second-order central-transition powder patterns. A line shape with an Density functional theory asymmetry parameter Z close to zero is easily identiﬁed. The Electronic structure calculations were carried out to relate high signal to noise ratio allowed visualization of the small but quadrupolar interaction parameters to the diﬀerent cation distinctive features extending from both sides of the spectrum conﬁgurations. The local electric ﬁeld gradients have been of the spectrum indicating the presence of a species with a high calculated with the ﬁrst-principles molecular-dynamics asymmetry parameter. The broad resonances are assigned to programme VASP,32–35 using density functional theory and 75 As resonances with an asymmetric ﬁrst coordination shell. the PAW method41,42 following the approach by Petrilli Based on a simple point charge model46 we calculate a et al.31 several convergence tests were carried out, in particular quadrupolar coupling constant of approximately 33 MHz to estimate the eﬀect of the semi-core states and compared for these coordinations. The asymmetry parameter is predicted with state-of-the-art quantum chemical calculations using to be Z = 1 for the As[Al2Ga2] coordination and Z = 0 for the DALTON.43 A detailed summary of the convergence test, As[Al1Ga3] and As[Al1Ga3] coordinations. The enormous molecular simulations on small model systems for AlGaAs width of the spectrum makes it diﬃcult to determine the and the choice of DFT functional, can be found in the chemical shift of these resonances with any accuracy. supplementary material. Convergence of the results with The spectra were ﬁtted using an evolutionary algorithm38 to respect to k-point sampling, kinetic energy cut-oﬀ of the plane deconvolute the signals into the contributions from each wave basis set, and lattice relaxation was checked as well. AlAs individual 75As site as is shown in Fig. 2. The diﬀerent has an experimental lattice spacing of 0.56695 nm and GaAs quadrupolar subspectra used as library spectra for ﬁtting the of 0.56614 nm, see ref. 21, thus the lattice mismatch for QCPMG spectra were calculated assuming ideal non-selective Al0.5Ga0.5As is r 0.1%. Relaxation of the structure resulted excitation in SIMPSON.39 The ﬁt with the lowest average cost This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
8.
View Online resonances experiencing only very small EFGs. Indeed the spectra show some spectral distortions around the center frequency due to truncation of the narrow lines. As the oﬀ-resonance behavior of the lines with small (o1 MHz) and large (430 MHz) quadrupolar interactions diﬀers, adding the oﬀ-resonance spectra somewhat aﬀects the shape of the spectrum. The broad resonances of the As[Al1Ga3],Downloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 As[Al1Ga3] and As[Al2Ga2] coordinations could be ﬁtted very well however, and gave consistent results in ﬁtting the spectra of both the Al0.297Ga0.703As and Al0.489Ga0.511As sample. The ﬁt parameters are summarized in Table 3. The eﬀective excitation diﬀers signiﬁcantly for the various sites at diﬀerent resonance oﬀsets.12,13 Therefore we question Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B the possibility to reliably quantify the relative intensities of the arsenic sites considering spectra obtained at diﬀerent resonance oﬀsets were added. Moreover, it is too time consuming to calculate the entire signal response, consisting of the 242 echoes, for each of the B2000 Cq and Z values, which are needed for the ﬁtting library, using actual excitation parameters. To get a reasonable estimate for the molar ratios of the diﬀerent arsenic coordinations, the on-resonance QCPMG spectra (i.e. with the excitation frequency in between the narrow lines) were ﬁtted for each sample. In this case the broadened line shapes were mimicked by using the average quadrupolar coupling constant and adding a large Gaussian broadening of 50 kHz. The intensities obtained in this ﬁt were scaled by the relative intensities obtained in a SIMPSON simulation of a single echo for each site using the actual rf ﬁeld strengths as used in the experiments. The results are given in Table 3. Comparing the intensities from this analysis to the relative intensities expected for random ordering of the Al and Fig. 2 (top) 75As absolute sum of all 24 frequency-stepped QCPMG spectra of Al0.297Ga0.703As (dotted line) obtained at 18.8 T and the Ga nuclei deviate for both the Al0.489Ga0.511As and the simulated spectrum of a GA-based ﬁt using a library of spectra Al0.297Ga0.703As with the discrepancies being largest for the simulated using the SIMPSON package (solid line). The ﬁve lower latter sample. In both QCPMG spectra the intensities of spectra show the contributions from each site. (bottom) The sum of all the As[Ga4] and As[Al4] resonances with small quadrupolar 22 frequency-stepped QCPMG spectra of Al0.489Ga0.511As together interactions seem to be substantially underestimated. with the ﬁtted result and the individual contributions of each site. The experimental SNR was E120 per frequency step accumulating 75 5400 scans. II. As Hahn-echo analysis Although the QCPMG experiments give good signal to noise ratios for the very wide 75As resonances, revealing even broad or w2 was found using the model with the least constraints, i.e. low intensity features at the edge of the lines, the quantiﬁcation using a Gaussian quadrupolar distribution in the Cq and a of the relative intensities in the spectra is considered to be single Z value. Although good line shapes are obtained, ﬁtting compromised. Therefore we attempted Hahn-echo experiments with a Gaussian distribution in Cq and Z does not have a at an elevated rf-ﬁeld strength to get easier processing and physical meaning. Therefore as has been discussed, we used calibration of the spectra. The experimental results, together the Czjzek distribution with d = 5 to describe the narrow with unrestrained ﬁts of these spectra are shown in Fig. 3 and 4 resonances and extended Czjzek distributions for the broad for Al0.297Ga0.703As and Al0.489Ga0.511As. Indeed the signal to resonances thus taking the eﬀect of the ﬁrst coordination shell noise of the x E 0.489 Hahn-echo was a factor 46 lower than on the EFG tensor into account. Based on some initial a corresponding QCPMG spectrum, but the main spectral simulations and the size of the quadrupolar coupling constant features are similar to those observed in the QCPMG spectra. of the As sites with a symmetric ﬁrst coordination shell, the The library ﬁles used for the GA analysis were obtained contribution of the higher coordination spheres was ﬁxed to from SIMPSON simulations of the Hahn echo using the 715 kHz in the ﬁts of the spectra. parameters as used in the experiments. As before, the The frequency stepped QCPMG experiment was designed to As[Ga4] site was ﬁtted with a ﬁxed Czjzek distribution obtain undistorted lineshapes from very broad quadrupolar with hCqi = 610 kHz and d = 5, the As[Al4] site with resonances at limited rf-ﬁeld strengths. Here we are faced with hCqi = 820 kHz and d = 5, and as ﬁxed input for the the presence of very broad sites with large quadrupolar distribution of the extended Czjzek distributions for the interactions and narrow lines for the As[Ga4] and As[Al4] As[AlnGa1Àn], n = 1,2,3 sites we used the average quadrupolar Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
9.
View Online Table 3 NMR parameters obtained from ﬁtting the experimental spectra. The reported conﬁdence intervals are standard deviations from 7 ﬁts. The relative intensity of each site is normalized to the echo maximum in the time domain. In the restrained ﬁt, the SCuAu order parameter was left free to ﬁt and converged to S = 0.01 Æ 0.01 and x = 0.483 Æ 0.004. The 75As quadrupolar coupling constant was calculated from the EFG by multiplication with a factor of 0.75925 MHz per 1020 V mÀ2. An increased w2 corresponds to a poorer ﬁt. Relative intensity x E 0.297 Relative intensity x E 0.489 Summed On-res. Hahn-echo Summed On-res. Site Hahn-echo QCPMG QCPMG S = 0a Hahn-echo S—ﬁtb QCPMG QCPMG S = 0aDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 As[Ga4] 0.14 Æ 0.01 0.047 0.24 0.089 Æ 0.01 0.071 0.028 0.071 As[Al1Ga3] 0.46 Æ 0.03 0.64 0.48 0.43 Æ 0.01 0.50 0.54 0.50 As[Al3Ga1] As[Al2Ga2] 0.39 Æ 0.02 0.31 0.26 0.42 Æ 0.01 0.37 0.41 0.37 As[Al4] 0.004 Æ 0.001 0.003 0.008 0.065 Æ 0.01 0.054 0.020 0.057 Quadrupolar coupling constant (MHz) Quadrupolar coupling constant (MHz) As[Al1Ga3] 33.2 Æ 0.1 33.2 Æ 0.1 33.4 33.3 Æ 0.1 33.3 Æ 0.1 33.3 Æ 0.1 33.4 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B As[Al3Ga1] As[Al2Ga2] 30.3 Æ 0.1 31.9 Æ 0.1 33.4 30.5 Æ 0.1 31.2 Æ 0.2 32.5 Æ 0.1 33.4 Additional ﬁtting parameters w2 0.57 0.74 0.98 2.14 1.02 Fitted line broadening (kHz) 5.0 11.8 2.0 12.4 12.4 8.0 4.0 a b Theoretical Intensities corresponding to SCuAu = 0 (eq. 6) Fit of the Hahn-echo data imposing the CuAu order parameter model. As an alternative we imposed the CuAu order parameter model in the ﬁtting procedure of the x E 0.489 spectrum, leaving the SCuAu free to ﬁt and the composition value x free to vary within 2%, which will constrain the ﬁve relative intensities. The latter was implemented to allow for experi- mental errors in the composition x, from the growth process. Fig. 4 shows the ﬁt of the Al0.489Ga0.511As spectrum. The best ﬁt was obtained for S = 0.01 and x = 0.483. Compared to the free ﬁt with w2 = 0.98 the w2 increased to 2.14, see Table 3. The restrained ﬁt imposes the relative intensities deﬁned by the long-range order parameter and it was observed that the least square deviation increased. Nevertheless, this restrained ﬁt is considered reasonable, since the spectra show no indication of long range order in the samples in accordance with X-ray data. Using the same approach the Al0.297Ga0.703As sample shows Fig. 3 The experimental 75As Hahn-echo of Al0.297Ga0.703As (dotted a very diﬀerent picture, however. In this case it proved line) obtained at 18.8 T together with the ﬁtted spectrum (solid line) impossible to ﬁt the relative intensities complying to an order using a genetic algorithm (see text). The ﬁve lower spectra show the parameter model. individual contributions from each arsenic site. Spectra were averaged To estimate the reproducibility of the ﬁt procedure, for 166 000 scans leading to an SNR B 80. synthetic spectra were generated with random noise of the same order of magnitude and with the same bandwidth as was coupling constant of the two symmetric sites hCqi = 715 kHz, visible in the experimental spectrum. The standard deviation the EFG principal values VZ0 and VZ1 from the ﬁrst coordination of the relative intensities due to white noise, did not exceed shell of these sites were left free to ﬁt. As is clear from the ﬁts 2%. The conﬁdence intervals for the relative intensities were of the x E 0.297 (Fig. 3) and 0.489 samples (Fig. 4), the determined from the standard deviation of seven diﬀerent ﬁts, spectral deconvolution using the Czjzek and extended Czjzek 1% error margin was added to each site to account for distributions works very well for all spectra. The quadrupolar systematic errors. The conﬁdence intervals are smaller for interaction parameters obtained from these Hahn-echo data the x B 0.489 sample, caused by the more distinctive shape are in good agreement with those obtained from the QCPMG of the spectrum. p1 and p3 were undistinguishable and data. The quadrupolar coupling constant for the As[Al2Ga2] considered as one intensity p1 + p3. site is slightly lower which is attributed to the less eﬃcient The spectra of both the Al0.489Ga0.511As and the excitation of the broad features at the edges of the Hahn-echo Al0.297Ga0.703As sample do not show distinct signs of long- spectra. The relative intensities obtained from the these spectra range order. The distributions in quadrupolar interaction diﬀer signiﬁcantly from those estimated from the on-resonance parameters clearly indicate positional disorder in the occupance QCPMG spectra. The intensities of the narrow lines seem of the Al and Ga sites in the higher coordination spheres of all much more realistic now, but the values obtained from the the arsenic in the lattice. Remarkably, however, the relative simulations still diﬀer from those expected for an order intensities of these sites do not comply with an S = 0 situation parameter model. using the order parameter model as used for the description of This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
10.
View OnlineDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B Fig. 5 (top) The theoretical relative intensities pn as a function of the CuAu order parameter S for x = 0.297 , see eqn (6) (solid lines). The experimental relative intensities expn of the Hahn-echo are plotted as vertical bars representing their conﬁdence intervals + 1% systematic model error per site. (bottom) x = 0.489. Fig. 4 (top) The experimental 75As Hahn-echo spectrum (18.8 T, 166 000 scans, SNR B 80) of AlxGa1ÀxAs, x = 0.489 (dotted line) performed for 71Ga and 69Ga at 14.1 T for the x B 0.297 together with the ﬁt (solid line). The ﬁve lower spectra show the sample. Here we focus on the 69Ga results because of its larger contributions from each site. (bottom) Restrained ﬁt imposing a CuAu quadrupolar moment, giving the largest sensitivity to electric order parameter model, where the S-parameter was left free to vary ﬁeld gradients. In the case of an ordered structure, or domains and the x could vary within 2%. The relative intensities ﬁtted to with high ordering, there should be a Ga resonance without S = 0.01 and x = 0.483. The ﬁve lower spectra show the contribution any quadrupolar broadening in the spectrum. In 69Ga static from the individual sites. spectrum only one (Gaussian) signal is present at B6 ppm with respect to GaAs. In a nutation experiment the line shape XRD data. Although a restrained ﬁt of the x E 0.489 sample is dependent on the ratio of the quadrupolar frequency nQ and did ﬁt to S = 0. For this sample the results show a similar the rf-ﬁeld strength n1. The nutation spectra in Fig. 6 show observation as that by Tycko et al.,22 i.e. that the relative rather featureless lines, as was also observed earlier for NMR intensities of diﬀerent C atom coordinations in x B 0.489 by Degen et al.21 This is attributed to the eﬀect AxB1ÀxC type materials can be used to set an upper limit to of a distribution in quadrupolar parameters and to some the long range order parameter in such materials. The ﬁtted extent the eﬀect of RF inhomogeneity. Degen et al. found a relative intensities for the x E 0.297 sample deviate strongly Cq = 520 kHz and Z 4 0.97 for x E 0.489. We ﬁtted the data from the order parameter model and could not be ﬁtted to any using Czjzek distributions with d ranging from 1 to 5 and for S (Fig. 5). It should be noted that, the order parameter model s = 100 to 600 kHz. It is veriﬁed that the simulated nutation as used here, only considers the average long range order and spectra for Z B 1 (dashed thin line), or a Czjzek distribution does not take any speciﬁc short range order into account. (solid line) do not diﬀer much. Although it was not possible to Therefore, it is worthwhile to explore further if the NMR uniquely ﬁt the nutation data to a speciﬁc model, the spectra spectra contain any information about local order on a nm clearly preclude the existence of a Ga site with a near zero scale. Short range ordering contains similar surroundings/sites quadrupolar interaction or/and low Z. This rules out the As[AlnGa4Àn] n = 0–4, but for n = 1,2,3 each surrounding has presence of highly ordered domains in this sample. a discrete set of tensor orientations (see Section DFT). An additional veriﬁcation of the absence of well-deﬁned Ga 69 sites in ordered structures comes from 69Ga static, MAS and III. Ga nutation and 3QMAS 3QMAS spectra. The 69Ga line width contains diﬀerent To independently verify the random distribution of Al and Ga contributions including quadrupolar and dipolar broadening over the lattice, a series of static nutation experiments were and broadening due to the exchange interaction.47 At 9.4 T the Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
11.
View OnlineDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B Fig. 6 Experimental 69Ga static nutation spectra obtained at 14.1 T Fig. 7 Sheared 69Ga 3QMAS spectrum obtained at 14.1 T. using diﬀerent rf ﬁeld strengths for Al0.297Ga0.703As (dashed thick A z-ﬁltered 3QMAS spectrum was acquired using rf-ﬁeld strenghts lines). The solid lines represent SIMPSON simulations of the nutation of 120 kHz and 20 kHz for the hard (5.4 respectively 1.8 ms) and spectra assuming a Czjzek25 distribution in the quadrupolar inter- selective (6 ms) pulses, respectively. The n1 dimension was scaled by action parameters. Shown is the best ﬁt using d = 5, hCqi = 2Ás = 9/34 to get an easy interpretable ppm scale. In this convention a 0.60 MHz. The dashed thin lines were calculated using Z = 1 and hypothetical resonance without quadrupolar interaction has the same Cq = 0.80 MHz. shift value in ppm on both axes. static Gaussian full width at half maximum (FWHM) is cost the number of conﬁgurations studied and hence 2.8 kHz, using 15 kHz Magic Angle Spinning (MAS), the the statistical quality of the EFG distributions is limited. shape remains Gaussian with a FWHM of B1.6 kHz. Moreover, only a few values of the order parameter S can The second order quadrupolar contribution to the linewidth be realized. This ‘‘supercell model’’ approach provides a is of the order of (3/64)Á(C2 /nz).48 With quadrupolar coupling q semi-quantitative understanding. In the second approach, constants up to B800 kHz this contribution is less than called the ‘‘multipole model’’, we exploit the additivity of B300 Hz. Therefore the main contributions to the linewidth EFGs in AlGaAs. This allows for calculating large numbers originates from a distribution in isotropic chemical shift of structures, high quality statistics and many values of S to be and/or exchange interaction. This is also clear from the 69Ga studied. In this part we restrict ourselves to a computation (3Q)MAS spectrum obtained at 14.1 T for Al0.297Ga0.703As with equal amounts of Al and Ga present. Finally, we will shown in Fig. 7. The broadening of the spectrum mainly show that the obtained distributions for S = 0 concur with the extends along the shift axis. From the position of the analytical result of the extended GIM, described by Le Caer ¨ center of gravity in both directions, d1 = À5.1 ppm and and Brand.26 d2 = À7.4 ppm, an average isotropic chemical shift diso = À6.0 ppm and an average quadrupolar induced shift I. Supercell models dqis = À1.45 ppm pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ was determined resulting a quadrupolar To approximate the distributions observed in the experimental product PQ ¼ CQ Á 1 þ Z2 =3 of 730 kHz in accordance with spectra of the x E 0.489 sample by theory, twelve structures the nutation data. Again there is no indication of a site with with x = 0.5 were simulated. Cubic-shape supercells were a well-deﬁned (small) quadrupolar coupling constant and used, containing 16 formula units in a 2 Â 2 Â 2 arrangement asymmetry parameter which would be expected for sites in of conventional zinc blende unit cells, i.e., Al16Ga16As32. Here ordered domains in the sample. we discuss the change in orientation of the tensors, as the occupation of the cation lattice goes from full CuAu ordering DFT Modeling to a more random arrangement. One structure was created with full CuAu ordering (SCuAu = 1) and one with partial high To gain more insight in how structural variations translate ordering, SCuAu = 0.875. Ten structural models were created into NMR parameters, in particular the quadrupolar inter- using random positioning of the Al and Ga cations, all with action and its distributions, we need to simulate many diﬀerent SCuAu r 0.25. The calculated principal z-axis of the EFG structures and relate these structures to the NMR parameters. tensor is plotted for each atom in Fig. 8. All atoms were kept It has been shown that a point charge model is not able at their ideal lattice positions. to properly predict the EFG distributions in these type of systems.49 A good model should rely on ﬁrst-principles input data. We address the problem in two ways: ﬁrst, we make Full order. In a fully ordered CuAu Al0.5Ga0.5As lattice, the ordered and randomized structural models using supercells, only 75As site present is As[Al2Ga2]. The principal z-axis of the with the compositions x = 0.5 and x = 0.3125 and calculate EFG tensor of this site always lies in the As x À y plane (under their EFGs with DFT. This approach also allows one to access an angle of 45 degrees). The in-plane orientation changes by the energetics of these models. Because of the computational 1801 between adjacent As layers. This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
12.
View Online structure, with a small distribution in the principal EFG z-axis direction for the n = 1,2,3 sites and a spread of DZ = Æ0.03. 8 of the 32 As atoms are n = 1,3 sites. As depicted in the ﬁgure, the Principal Axis System (PAS) of the As[Al1Ga3] (n = 1) or As[Al3Ga1] (n = 3) EFG tensors have their z-axis oriented along any body diagonal of a cube, i.e. in one of 4 possible directions. The main diﬀerence betweenDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 As[Al3Ga1] and As[Al1Ga3] is the positive/negative sign of the quadrupolar coupling. The principal z-axis of an As[Al2Ga2], n = 2 EFG tensor has 6 possible orientations along all face diagonals of a cube. Random. In a random lattice the three sites with n = 1,2,3 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B occur with diﬀerent relative intensities and the EFG distribution within all sites is much stronger. Ten diﬀerent random models were used to estimate the distributions in the tensor values. In Fig. 9 we approximate the distributions for the n = 1 and n = 3 sites with a Gaussian-type distribution as used by Jager¨ and coworkers.23 Although the simulated EFG data roughly follow that of a Gaussian distribution, the statistics do not allow a deﬁnite conclusion on the shape of the distribution, i.e. we cannot decide whether it is a Gaussian. Indeed, on physical grounds we do not expect a Gaussian distribution. Evidently we need a model that allows for higher quality statistics (see next section). As[Al4] and As[Ga4] sites are even more rare in the generated structures, so we do not attempt to ﬁt their distributions with any functional form. The averages and standard deviations of the Vzz and Z distributions for x = 0.5 are listed in Table 5. Similar calculations were carried out for the composition with x = 0.3125 as summarized in Table 6. Inspecting the tables, we see that for both compositions the agreement of the average 75 As Vzz and Z with the experimental results is reasonable for the random models, for all n = 0–4. For the hVzzi of the n = 0 and n = 4 sites the relative diﬀerence between calculation and experiment is larger, with calculations overestimating the average EFGs. We have to keep in mind that these EFGs are very small, since they are caused by distant coordination shells. The neglect of the contributions of the arsenic core states might explain this discrepancy (see supplementary Fig. 8 2 Â 2 Â 2 (conventional unit) cells of a Al0.5Ga0.5As lattice containing 64 atoms. The horizontal layers from bottom to top are Al (blue), As (green), Ga (red), As, Al, As, Ga, As. The arrows display the direction of the Vzz principal EFG tensor direction for each atom. (top) fully ordered lattice with SCuAu = 1, (middle) partially ordered lattice with SCuAu = 0.875, (bottom) randomly ordered lattice with SCuAu r 0.25. Fig. 9 Vzz and Z distributions for As[Al1Ga3] and As[Al3Ga1] sites. Solid line: DFT calculations for 10 random supercells of the Al0.5Ga0.5As lattice. The dotted line shows a Jager type23 Gaussian ¨ Partial order. Swapping only two cations in a 2 Â 2 cell distribution with hCqi = 33.0 MHz, a HWHM = 0.4 MHz and results in a partially disordered but still highly ordered Z = 0.03. Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
13.
View Online Table 4 Total energy of the AlxGa1–xAs supercells, depending on the This procedure is very fast, as it obviates the need for a composition and order parameter. The partially ordered structure for separate DFT calculation for each diﬀerent atomic conﬁguration. x = 0.5 is displayed in Fig. 8. ‘‘Random 1–10’’ denotes 10 diﬀerent near random structures with low order parameter S. For Al10Ga22As32 It can be somewhat reﬁned at negligible computational cost. with x = 0.3125 ‘‘order 1’’ has a relatively high ordering, with full Ga The distributions P(|Vzz|,Z) are modeled as a function of the occupation of one layer and 2 identical cations in the farthest layer. order parameter SCuAu. On the computer we generate many, ‘‘order 2’’ has full Ga occupation of one layer and 2 identical cations in 3 Â 106, conﬁgurations by randomly placing cations in the the nearby layer. ‘‘order 3’’ has 5 identical cations in layers 1 and 2 (small cluster) 4 Â 4 Â 4 unit cell. For each conﬁguration we determine theDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 order parameter SCuAu from the deﬁnition in eqn (1) and then Total energy (eV/cell) SCuAu Vzz and Z for all atoms. Counting the number of occurrences Al16Ga16As32 of the (Vzz,Z) values then yields the quadrupolar distributions Fully ordered CuAu À283.098 1 as displayed in Fig. 11. Partially ordered À283.100 0.875 Now let us consider the assumptions that go into this Random 1–10 À283.123 – À283.150 0 – 0.25 Al10Ga22As32 procedure. Suppose we interchange one Al for a Ga atom in Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B Order 1 À277.186 0.5 AlxGa1–xAs. In ﬁrst order only the polar bonds between the Order 2 À277.214 0.375 Al/Ga and its 4 neighboring As are aﬀected. The charge Order 3 À277.163 0 Random 1–10 À277.163 – À227.188 0 – 0.375 redistribution preserves the local tetrahedral symmetry, hence the leading order induced charge moment will be that of an octopole. These octopole (and higher) terms will give rise to an information). For 69Ga the agreement for x = 0.5 also seems electric ﬁeld at nearby As sites. The ﬁeld, in turn, will be good, at least as far as the average Vzz is concerned. The screened by the other atoms on the AlxGa1–xAs lattice. This average 27Al Vzz is considerably underestimated in these screening is described by the microscopic dielectric function calculations, however. This is probably also related to the e(r,r 0 ). In our approach, we implicitly assume this function is neglect of core contributions (see supplementary information). independent of the local chemical composition (indeed this Table 4 (upper part) summarizes the calculated total is our central assumption). This is reasonable as the energies for the (x = 0.5) structures displayed in Fig. 8. The (macroscopic) dielectric constants of AlAs and GaAs do not random structures all have lower total energy than the fully diﬀer much (eN = 8.2 respectively eN = 10.8).50 We have also and partially ordered structures. The energy diﬀerences are checked this assumption by recalculating the EFGs with DFT small: DE E 0.04 eV/64 atoms = 0.6 meV/atom. So we do not for a limited number of random conﬁgurations (in smaller observe a signiﬁcant thermodynamic driving force for super cells). Note that we also neglect the eﬀect of local atomic ordering. relaxations. This is justiﬁed as the lattice match between AlAs For the x = 0.3125 composition perfect CuAu ordering is and GaAs is nearly perfect and structural relaxations are not possible. Therefore, we compare the random structures very small. with several ordered models with S a 1. One of the ordered In Fig. 10 the arsenic Vzz as obtained by DFT in the models has the lowest total energy, but the diﬀerences in AlGa255As256 and Al255GaAs256 super cells is plotted as a energy with other structures are very small. Keeping in mind function of the distance to respectively the Al or Ga atom. that there is also an entropic contribution favoring disorder, Note that only beyond the third As shell the contributions to we again cannot conclude that there is a tendency towards the Vzz become very small. This occurs at a distance well below ordering. half of the size of the super cell (2.25 nm/2). So our super cell is chosen suﬃciently large that spurious contributions from II. Multipole model periodic images are avoided. As good statistics requires a large number of conﬁgurations, Remarking that the screening is dominated by the atoms in we need a very fast method to calculate the EFGs for each new the ﬁrst shell, we can improve our modeling of the conﬁguration. Below we ﬁrst describe this method, provide As[Al4] sites. Based on a DFT calculation with a single Ga a physical justiﬁcation, give details on generation of the (Al255GaAs256, called ‘‘Ga in a sea of Al’’) we correctly conﬁgurations and analyze the results. This model reproduces describe the screening by the ﬁrst shell, whereas with the the absolute EFG tensor values with an accuracy of B10%, calculation based on AlGa255As256 (‘‘Al in a sea of Ga’’) all compared to an independent direct DFT calculation. ﬁrst shell atoms are Ga. The latter would be more appropriate We start with a single DFT calculation on a large cubic for the As[Ga4] sites. More information on the diﬀerence super cell consisting of 4 Â 4 Â 4 conventional zincblende unit between the ‘‘Ga in a sea of Al’’ and ‘‘Al in a sea of Ga’’ cells. All cations are Ga, except for one, i.e., the cell has results can be found in the supplementary information. composition AlGa255As256. The DFT calculation yields the As each conﬁguration of Al128Ga128As256 yields a speciﬁc EFG tensors for all 256 As atoms so that we know the As EFG EFG and Z, an EFG distribution can be constructed relatively as a function of rAsGa, the vector from Ga to As. For any fast from many occurrences with similar order parameters possible conﬁguration of any possible cell with composition SCuAu. Conﬁgurations that do not match the ‘‘stoichiometry’’ AlnGa(256–n)As256 we calculate the EFGs by multiple addition: constraint Al128Ga128As256 are discarded. The conﬁgurations For each Ga we add its contribution to the As EFGs are sorted by SCuAu that is calculated using eqn (1). at displacements rAsGa using the result of the single DFT Fig. 11 shows the variation in the As[AlnGa4–n] EFG calculation. Once the contributions due to all Ga’s have distributions, as calculated with the ‘‘multipole model’’ for been added, the As Vzz and Z are obtained by diagonalization. diﬀerent CuAu order parameters SCuAu. As S becomes larger, This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
14.
View Online The n = 2, i.e., Z(0) = 1 ﬁt in Fig. 13 cannot be obtained with a simpliﬁed analytical expression, such as eqn 61 in Le Caer ¨ and Brand. This distribution was obtained numerically, by integrating eqn (10) over all three Euler angles (0 r a o 2p, 0 r b o p, 0 r g o 2p). We also modeled the EFG distributions of the Ga and Al sites for the disordered S = 0 situation using the additivityDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 model of the tensor values, applying the ‘‘Al in a sea of Ga’’ or ‘‘Ga in a sea of Al’’ approach. These distributions appeared to be more complex and do not follow the regular or extended Czjzek distribution. For Ga the overlap with a Czjzek distribution with d = 5 is displayed in Fig. 14. Even Fig. 10 Principal EFG component Vzz for 75As as a function of the though the cations are randomly positioned, the calculated Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B distance to a Ga or Al atom in the AlGaAs lattice. The data were distribution is more structured than a Czjzek with d = 5. calculated using a Al255GaAs256 super cell, referred to as ‘‘Ga in a sea We attribute this to the fact that for gallium the distribution of Al’’ (dotted line) or a AlGa255As256 (solid line) super cell, ‘‘Al in a mainly originates from the closer, second shell. This is sea of Ga’’. In the ﬁrst shell Vzz (not shown) attains values of closer than the case of the arsenic n = 0 and n = 4 sites, where Æ43.6 Â 1020 V mÀ2. The curves are a guide to the eye. the ﬁrst and second shell are isotropic. So we conclude that the eﬀect of the closer second shell cannot be modeled with a fully in general, the average As Vzz and Z values increase. In the random model such as the Czjzek distribution with d = 5. lower S range, the distributions are rather insensitive to S (compare the S = 0 and S = 0.5 curves). Increasing S to 0.5, all As Vzz distributions become more symmetric, except IV. Comparing theory and experiments for As[Al2Ga2] which develops a pronounced asymmetry. For The average EFG values can be predicted well using our DFT higher S, a pattern with shoulders and ‘‘spikes’’ develops. A approach as implemented in the VASP package. For arsenic, similar observation was described analytically in the work of we approach the experimental results quite satisfactory: For Le Caer et al.26 (their Fig. 4 and 5). The quadrupolar ¨ As[Al1Ga3], As[Al3Ga1] and As[Al2Ga2] sites the discrepancies distributions for the n = 0,4 sites can be described with Czjzek between theory and experiment for e.g., hVzzi (hCqi) are distributions for d = 5 and S = 0. Vzz of the n = 1–3 sites are substantially below 10% for both sample compositions dominated by the atoms in the ﬁrst coordination shell of the x = 0.5 and x = 0.3125. For the As[Al4] and As[Ga4] sites, arsenic and the average Vzz typically changes by B3% going the discrepancies are somewhat larger. It should be noted, from S = 0 to S = 1 and the distribution narrows. however, that these EFGs are two orders of magnitude As expected, the n = 0 and n = 4 As site provide a much smaller. The diﬀerences could be due to small errors arising more sensitive probe to the degree of disorder, and a from the neglect of the response of (deep) core electrons. The concomitantly weaker EFG (Fig. 12). The degree of (dis)order limited number of random supercell models that could be has an even more dramatic impact on the Ga distributions: not generated do not allow to make predictions about the exact only does the average Vzz increase from B1.0 Â 1020 V mÀ2 shape of the distributions P(Vzz,Z), however. For x = 0.5 for S = 0 to B1.8 Â 1020 V mÀ2 for SCuAu = 1 (an 80% we showed that the combined EFG distribution of the increase) but also the width of the distribution is reduced by As[Al1Ga3]/As[Al3Ga1] sites (Fig. 9) still had insuﬃcient almost an order of magnitude. The wild oscillations in these statistical quality. This distribution was derived from an Z patterns might be attributed to an insuﬃcient number of average of 176 + 113 = 309 diﬀerent As sites, see Table 5. conﬁgurations, as the number of conﬁgurations decreases with For the As[Ga4] and As[Al4] sites we can only average 17 and increasing S. 14 conﬁgurations respectively, so it is really impossible make any statement on the shape of the distribution function III. The extended GIM model P(Vzz,Z) based on this data. We will now focus on the simulations for S = 0. As shown in The multipole model with x = 0.5 was based on 3 Â 106 the upper ﬁgure of Fig. 13, for a lattice with random order, the conﬁgurations, where each conﬁguration was constructed out distribution in the quadrupolar parameters of As[Ga4] and of 256 As atoms. This allows for reliable statistics, also for the As[Al4] derived from the ‘‘multipole model’’ perfectly match a relatively rare As[Al4] and As[Ga4] sites. The additional Czjzek distribution with d = 5 and an average quadrupolar approximations result in some errors, but all (n = 0–4)Vzz constant s. Such distributions are isotropic and rotation averages are well within the expected B10% of the supercell invariant. The quadrupolar distributions obtained for the models. The data obtained from the As[Al4] site seems to n = 1,2,3 sites for the S = 0 structures could be matched deviate more, but note that the estimated RMS error in when a deﬁned ﬁrst shell tensor was added the distributions in the average, obtained with the supercell models, is pﬃﬃﬃﬃﬃ EFG due to the disorder in the higher coordination sphere as 0:33 MHz= 14 ¼ 0:09 MHz $ 8%. With the multipole described earlier. In fact, these distributions also matched the model, the discrepancy between theory and experiment for analytical extended GIM as described by Le Caer and ¨ As[Al4] is reduced to B15%. The As[Ga4] has, unfortunately, Brand.26 The n = 1 and n = 3 distributions have Z(0) = 0 increased a bit to B25%. As these EFGs are very weak, we and match with their eqn 61, see bottom ﬁgure of Fig. 13. think these results are very reasonable. Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
15.
View OnlineDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B Fig. 11 Vzz (left) and Z (right) distributions of the diﬀerent arsenic sites in Al0.5Ga0.5As for diﬀerent order parameters SCuAu = 0,0.5,0.75,0.94 as obtained from DFT-based modeling of a Al128Ga128As256 super cell. The distribution in the quadrupolar parameters for the As[Al4] site was simulated using the ‘‘Ga in a sea of Al’’ model, all other sites were calculated using the ‘‘Al in a sea of Ga’’ approach. The main advantage of the multipole model is that we can Conclusions now study the distribution functions themselves, even for the diﬃcult sites As[Al4] and As[Ga4]. We found (Fig. 13) that A judicial choice of rf-coil diameter makes it possible to the latter are accurately described by Czjzek distributions observe 75As spectra from thin ﬁlm material of AlGaAs with d = 5. Thus we provide a ﬁrst-principles basis to grown by MOCVD. Reducing the coil diameter provides the support this model. Using these results to describe the sensitivity to study the limited amount of material available ‘‘amorphous’’ background, we then ﬁnd that the EFG from a single ﬁlm. Additionally the small diameter of the coil distributions of the As[Al1Ga3], As[Al3Ga1] and As[Al2Ga2] enables the generation of rf-ﬁelds large enough to eﬃciently sites are all accurately described by the extended Czjzek excite the entire bandwidth of the arsenic spectrum. Frequency- distribution. stepped QCPMG spectra and single Hahn-echo experiments This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
16.
View OnlineDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B Fig. 12 Vzz (left) and Z (right) distributions at the Al and Ga sites in Al0.5Ga0.5As for diﬀerent order parameters SCuAu = 0,0.5,0.75,0.94 and 1 as obtained from DFT-based modeling in a Al128Ga128As256 super cell. For S = 1 all occurrences have Z = 0. The Ga distribution was simulated using ‘‘Al in a sea of Ga’’. The Al distribution was simulated using the ‘‘Ga in a sea of Al’’ model. both reveal the presence of ﬁve resonances assigned to order present in both samples. The structural disorder in the As[AlnGa1–n], n = 0–4 with NMR parameters mostly depending occupancy of the Al/Ga sites is also reﬂected in the distributions on the symmetry of the ﬁrst coordination shell. The quadrupolar of the quadrupolar interaction parameters of the As sites. The coupling constant varies from less than 1 MHz for the symmetric As[Al4] and As[Ga4] sites have ﬁnite quadrupolar symmetric n = 0 and n = 4 coordinations, to over 30 MHz interactions with a distribution which can be described by a for the asymmetric n = 1,2,3 coordinations. Using an Czjzek distribution with uncorrelated Gaussian distributions evolutionary algorithm, the spectra can be decomposed into in the ﬁve independent electric ﬁeld gradient tensor values. the individual contributions from the diﬀerent As resonances. This reﬂects the random disorder in the higher coordination The frequency-stepped QCPMG data allow the most accurate spheres of these Arsenic sites which is isotropic and rotation determination of the quadrupolar interaction parameters; this invariant. For the As sites As[AlnGa1–n], n = 1,2,3 with a is of particular importance for the As[Al2Ga2] site whose mixed ﬁrst coordination shell, the electric ﬁeld gradients can be low intensity discontinuities from the Z = 0 second-order described by a summation of the EFG of the ﬁrst coordination quadrupolar powder pattern at the edge of the spectra are sphere to a Czjzek distribution resulting from the disorder in most pronounced in the QCPMG spectra. These spectra, the higher coordination spheres. This ‘‘background’’ Czjzek containing resonances from sites with small and large distribution is identical to the one obtained for the symmetric quadrupolar interactions can not produce reliable relative As[AlnGa1–n], n = 0,4 sites. intensities for the diﬀerent sites, however, due to the varying Field dependent 69Ga MAS NMR data, nutation and excitation eﬃciencies for the diﬀerent sites at varying resonance 3QMAS spectra of both AlxGa1–xAs (x = 0.489 or oﬀsets. The quadrupolar interaction parameters extracted x = 0.297) samples did not show the presence of Ga species from the Hahn-echo experiments are in accordance with those with a zero or very small quadrupolar interaction as would be obtained from the QCPMG data, except for the As[Al2Ga2] expected in the case of formation of ordered structures site that comes out slightly smaller. As expected the Hahn-echo supporting the conclusion of random ordering. experiments are less sensitive compared to the QCPMG data. DFT calculations of the electric ﬁeld gradient tensors based The advantage of the Hahn-echo data is that it is possible to on the PAW method implemented in VASP are in good determine the relative intensities of the As sites. agreement with the experimental data. As the lattice constants Imposing an order parameter model on the ﬁts gives a of AlAs and GaAs are nearly equal and their dielectric satisfactory solution of S = 0 for the Al0.489Ga0.511As sample, constants are very similar it is possible to calculate the eﬀects meaning the Al and Ga nuclei are randomly distributed of structural disorder in AlGaAs lattices based on calculations over their lattice sites. For the Al0.297Ga0.703As material no of a single Al255GaAs256 and AlGa255As256 supercell. From satisfactory ﬁt using the order parameter model could be these calculations the eﬀect of a Ga or Al on a speciﬁc As can obtained. These results indicate that there is no long-range be calculated and these contributions can be used in an Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
17.
View OnlineDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 Fig. 14 Simulated probability density function in the quadrupolar parameters of gallium, for S = 0 in a Al0.5Ga0.5As lattice. The solid Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B lines show a Czjzek distribution with s = 230 kHz and d = 5 for 69Ga. up to the 7th coordination shell, with the ﬁrst three shells being most dominant. Our ﬁndings of random cation arrangement for x E 0.297 and x E 0.489 agrees with earlier studies. Degen et al. found a short-range parameter S B 0–0.2 for similar samples on the bases of the intensities of the two symmetric As sites, with n = 0,4. Most studies of long-range order in these semi- conductors claim that the order parameter is quite small S o 0.05, indicating that clusters of similar ordering are not linked throughout the entire sample. Our data do not ﬁt very well using a long-range order parameter model even for S = 0. This might indicate that some short range order exists. Indeed, long and short-range order parameters do not have to be in the same range. Interrupted Al/Ga strings are observed in AlGaAs in an XSTM study.10 They ﬁnd a volume fraction of Al strings of only B0.3% for x = 0.15. The presence of Al strings would be observed in our resolved 75As spectra, if the volume fraction of strings is suﬃcient, roughly 41%. Besides sensitivity, an additional problem for analyzing powdered NMR data is that the distribution in EFG is convoluted with the powder distribution. The EFG tensors of the As[AlnGa1–n], Fig. 13 Overlayed contour plots of the probability density function in n = 1,2,3 sites have distinct orientations which are modulated quadrupolar coupling parameters P(Vzz,Z) generated from DFT by speciﬁc order or disorder in the higher coordination shell. calculations and using the analytical expression from Czjzek25 and Therefore more subtle studies of potential local order in these Le Caer and Brand.26 The dotted lines are the DFT-derived data using the multipole model for S = 0 of As[Ga4] (more noisy lines, top plot), materials would require the possibility to study a single As[Al2Ga2] (middle) and As[Al1Ga3]/As[Al3Ga1] (bottom). The solid oriented ﬁlm, which demands a further increase in volume lines show the Czjzek distribution with an average ﬁeld gradient of sensitivity. Miniaturization is a key concept here. We have 1.19 Â 1020 V mÀ2 and d = 5 (top), the extended Czjzek distribution recently shown advances in this area, using stripline based and a ﬁrst shell tensor VZ1 = 33.1 MHz, Z(0) = 1 (middle) and micro-coil detectors.14 VZ0 = 33.1 MHz Z(0) = 0 (bottom). All DFT calculations are based on the ‘‘Ga in sea of Al’’ approach. Acknowledgements additive manner when generating large numbers of random or The authors would like to thank J. van Os and G. Janssen for partly ordered structures. The distribution in quadrupolar technical support; M. Voncken for providing the AlGaAs parameters of the As sites derived from these analyses for samples; A. Lipton for his assistance on the Simpson discussion randomly ordered materials perfectly match those from the forum; A. Brinkmann and R. Siegel for experimental help and Czjzek (Gaussian isotropic) models used to describe the for the assistance with SIMPSON; C. Degen for aiding with experimental data. The Ga DFT simulations for S = 0 nearly the formulas to determine the intensities of the sites and match a Czjzek type distribution with d = 5, but the distribution S. Vasa for stimulating discussions. The DFT study is part is more complex. In general the calculations predict a shift of the research program of the ‘‘Stichting voor Fundamenteel and narrowing of the distribution in quadrupolar coupling Onderzoek der Materie (FOM)’’. Financial support from the constant with increasing order parameter. Furthermore the Nederlandse Organisatie voor Wetenschappelijk Onderzoek calculations show that there is an inﬂuence on the local EFG (Netherlands Organization for Scientiﬁc Research, NWO) is This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
18.
View Online Table 5 EFG simulations of Al0.5Ga0.5As compared to experimental results from Degen et al.21 and to the results of this study. The numbers A(C)n ﬃ represent A = average Cq value in MHz, C = standard deviation of the distribution in MHz, n = number of occurrences in the model. pﬃﬃ (C= n represents the accuracy of the mean value in MHz), ‘‘—’’ non-existing entries. The DFT calculations for the super cell models were carried out in a 2 Â 2 Â 2 unit cell, with 32 arsenic, and a total of 32 (aluminium and gallium) atoms. 10 super cells were used for x = 0.5 Theory (x = 0.5) Experiment (x E 0.489) Ordered CuAu Supercell models Multipole model S=1 SB0 S=0 Single value ﬁt21 This studyDownloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 Cq(MHz) 69 Ga 0.20 (0) 16 0.54 (0.20) 160 0.46 0.52 Æ 0.02 Al 0.046 (0) 16 0.16 (0.06) 160 0.18 0.083 Æ 0.007 As[Ga4] — 0.71 (0.23) 17 0.40c 0.61 Æ 0.020 0.61ac As[Al4] — 1.07 (0.33) 14 0.42c 0.82 Æ 0.050 0.82ac As[Al1/3Ga3/1] — 32.90 (0.59) 176 33.0ec 49 33.3 Æ 0.1ec As[Al2Ga2] 34.7 (0) 32 33.20 (3.07) 113 33.1ec 49 32.5 Æ 0.1ec Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B Z 69 Ga 0 0.62 (0.25) 0.63 40.97 Al 0 0.57 (0.28) 0.64 40.96 As[Ga4] — 0.63 (0.21) 0.61 40.97 0.66 As[Al4] — 0.66 (0.28) 0.61 40.88 0.66 As[Al1/3Ga3/1] — 0.03 (0.02) 0.03 0.03 As[Al2Ga2] 0.93 (0) 0.94 (0.02) 0.98 0.98 c Czjzek distribution with hCqi = 2.0Ás for d = 5; ac Assumed Czjzek distribution with d = 5 and Cq from the nutation data from ref. 21; ec Extended Czjzek distribution. Note that the compared values are average EFGs and not ﬁrst shell EFGs, although they do not diﬀer much. Table 6 EFG simulations of Al0.3Ga0.7As compared to the experimental results. The left column displays the results from a single simulation with the highest ordering, the second column displays the result from 3 partially ordered simulations, the third column from 11 random simulations Theory (x = 0.3125) Ordered CuAu Part. ord. Supercell models SCuAu = 0.375 SCuAu = 0.125 SB0 Experiment (x E 0.297) Cq (MHz) 69 Ga 0.54 (0.14) 22 0.47 (0.19) 66 0.45 (0.20) 242 0.69 Æ 0.10m 27 Al 0.14 (0.06) 10 0.09 (0.05) 30 0.14 (0.06) 110 As[Ga4] 0.81 (0.35) 12 0.75 (0.25) 28 0.89 (0.29) 68 0.61ac As[Al1/3Ga3/1] 33.1 (0.27) 8 33.1 (0.37) 24 32.97 (0.55) 180 33.2 Æ 0.1ec As[Al2Ga2] 34.5 (0.71) 12 34.6 (0.74) 44 33.36 (0.75) 102 30.3 Æ 0.1ec Z Ga 0.62 (0.30) 0.71 (0.26) 0.61 (0.25) 0.67 Al 0.40 (0.25) 0.22 (0.27) 0.55 (0.28) As[Ga4] 0.47 (0.26) 0.43 (0.23) 0.61 (0.23) 0.67 As[Al1/3Ga3/1] 0.04 (0.02) 0.03 (0.02) 0.03 (0.02) 0.03 As[Al2Ga2] 0.90 (0.03) 0.90 (0.03) 0.94 (0.02) 0.98 m ec MQMAS and nutation. Extended Czjzek distribution. acknowledged for sponsoring the solid-state NMR facility for 7 A. van Niftrik, G. Bauhuis and J. J. Schermer, J. Cryst. Growth, advanced materials science where the NMR experiments were 2006, 289, 48–54. 8 A. R. Smith, K. Chao, C. K. Shih, Y. C. Shih and B. G. Streetman, performed and the Stichting Nationale Computerfaciliteiten Appl. Phys. Lett., 1994, 64, 478. (National Computing Facilities Foundation, NCF) for the use 9 A. R. Smith, K. Chao, C. K. Shih, K. A. Anselm, A. Srinivasan of supercomputer facilities. and B. G. Streetman, Appl. Phys. Lett., 1996, 69, 1214–1216. 10 A. Heinrich and M. Wenderoth, Phys. Rev. B: Condens. Matter Mater. Phys., 1999, 59, 10296–10301. References 11 S. Adachi, Properties of Aluminium Gallium Arsenide, Institution of Engineering and Technology, 1993. 1 G. P. Srivastava, J. L. Martins and A. Zunger, Phys. Rev. B: 12 A. P. M. Kentgens, J. J. M. Lemmens, F. M. M. Geurts and Condens. Matter, 1985, 31, 2561–2564. W. S. Veeman, J. Magn. Reson., 1987, 71, 62–74. 2 G. B. Stringfellow and G. S. Chen, J. Vac. Sci. Technol., B, 1991, 9, 13 A. Samoson and E. Lippmaa, J. Magn. Reson., 1988, 79, 2182–2188. 255–268. 3 A. Gomyo, T. Susuki and S. Iijima, Phys. Rev. Lett., 1988, 60, 14 A. P. M. Kentgens, J. Bart, P. J. M. van Bentum, A. Brinkmann, 2645–2648. E. R. H. Van Eck, J. G. E. Gardeniers, J. W. G. Janssen, P. Knijn, 4 S. Froyen, A. Zunger and A. Mascarenhas, Appl. Phys. Lett., 1996, S. Vasa and M. H. W. Verkuijlen, J. Chem. Phys., 2008, 128, 68, 2852–2854. 052202. 5 C. Krahmer, M. Philippens, M. Schubert and K. Streubel, J. Cryst. 15 J. A. Tang, J. D. Masuda, T. J. Boyle and R. W. Schurko, Growth, 2007, 298, 18–22. ChemPhysChem, 2006, 7, 117–130. 6 T. S. Kuan, T. F. Kuech and W. I. Wang, Phys. Rev. Lett., 1985, 16 F. H. Larsen, I. Farnan and A. S. Lipton, J. Magn. Reson., 2006, 54, 201–204. 178, 228–236. Phys. Chem. Chem. Phys. This journal is c the Owner Societies 2010
19.
View Online 17 F. H. Larsen and N. C. Nielsen, J. Phys. Chem. A, 1999, 103, 32 G. Kresse and J. Hafner, Phys. Rev. B: Condens. Matter, 1993, 47, 558. 10825–10832. 33 G. Kresse and J. Hafner, Phys. Rev. B: Condens. Matter, 1994, 49, 18 F. H. Larsen, H. J. Jakobsen, P. D. Ellis and N. C. Nielsen, 14251. J. Magn. Reson., 1998, 131, 144–147. 34 G. Kresse and F. J., Comput. Mater. Sci., 1996, 6, 15. 19 A. Medek, J. S. Harwood and L. Frydman, J. Am. Chem. Soc., 35 G. Kresse and F. J., Phys. Rev. B: Condens. Matter, 1996, 54, 1995, 117, 12779–12787. 11169. 20 B. D. Cullity, Elements of X-ray diﬀraction, Addison-Wesley, 36 E. Yablonovitch, T. Gmitter and J. P. Harbison, Appl. Phys. Lett., Reading, MA, 2nd edn, 1978. 1987, 51, 2222–2224. 21 C. Degen, M. Tomaselli, B. H. Meier, M. M. A. J. Voncken and 37 M. E. Smith and E. R. H. van Eck, Prog. Nucl. Magn. Reson.Downloaded by RADBOUND UNIV. NIJMEGEN UNIVERSITEITSBIBLIOTHEK on 04 August 2010 A. P. M. Kentgens, Phys. Rev. B: Condens. Matter Mater. Phys., Spectrosc., 1999, 34, 159–201. 2004, 69, 193303. 38 W. L. Meerts and M. Schmitt, Int. Rev. Phys. Chem., 2006, 25, 22 R. Tycko, G. Dabbaghand, S. R. Kurtz and J. P. Goral, Phys. Rev. 353–406. B: Condens. Matter, 1992, 45, 13452–13458. 39 M. Bak, J. T. Rasmussen and N. Nielsen, J. Magn. Reson., 2000, 23 C. Jager, G. Kunath, P. Losso and G. Scheler, Solid State Nucl. ¨ 147, 296–330. Magn. Reson., 1993, 2, 73–82. 40 T. Vosegaard, A. Malmendal and N. C. Nielsen, Monatsh. Chem., 24 R. H. Meinhold, R. C. T. Slade and R. H. Newman, Appl. Magn. 2002, 133, 1555–1574. Reson., 1993, 4, 121–140. 41 P. E. Blochl, Phys. Rev. B: Condens. Matter, 1994, 50, 17953. ¨ Published on 02 August 2010 on http://pubs.rsc.org | doi:10.1039/C003624B 25 G. Czjzek, J. Fink, F. Gotz, H. Schmidt, J. M. D. Coey, 42 G. Kresse and D. Joubert, Phys. Rev. B: Condens. Matter Mater. J. P. Rebouillat and A. Lienard, Phys. Rev. B: Condens. Matter, Phys., 1999, 59, 1758. 1981, 23, 2513–2530. 43 DALTON, a molecular electronic structure program, Release 2.0 26 G. Le Caer and R. A. Brand, J. Phys.: Condens. Matter, 1998, 10, ¨ (2005), see http://www.kjemi.uio.no/software/dalton/dalton.html. 10715–10774. 44 J. P. Perdew, K. Burke and M. Ernzerhof, Phys. Rev. Lett., 1996, 27 H. J. Stockmann, J. Magn. Reson., 1981, 44, 145–158. ¨ 77, 3865. 28 J.-B. d’Espinose de lacaillerie, C. Fretigny and D. Massiot, 45 C. Degen, PhD thesis, ETH Zurich, 2005. J. Magn. Reson., 2008, 192, 244–251. 46 G. Engelhardt and H. Koller, Magn. Reson. Chem., 1991, 29, 29 G. Le Caer, B. Bureau and D. Massiot, J. Phys.: Condens. Matter, ¨ 941–945. 2010, 22, 065402. 47 O. H. Han, H. K. C. Timken and E. Oldﬁeld, J. Chem. Phys., 1988, 30 P. Blaha, K. Schwarz and P. Herzig, Phys. Rev. Lett., 1985, 54, 89, 6046. 1192. 48 A. P. M. Kentgens, Geoderma, 1997, 80, 271–306. 31 H. M. Petrilli, P. E. Blochl, P. Blaha and K. Schwarz, Phys. Rev. B: ¨ 49 S. Wei and A. Zunger, J. Chem. Phys., 1997, 107, 1931–1935. Condens. Matter Mater. Phys., 1998, 57, 14690. 50 Z. H. Levine and D. C. Allan, Phys. Rev. Lett., 1991, 66, 41–44. This journal is c the Owner Societies 2010 Phys. Chem. Chem. Phys.
Be the first to comment